HAL Id: hal-02042582
Submitted on 5 Mar 2019
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
developed mechanical energy for bone remodeling using a statistical reconstruction method
A. Sheidaei, M. Kazempour, A. Hasanabadi, F. Nosouhi, Martine Pithioux, Yves Remond, Daniel Georges
To cite this version:
A. Sheidaei, M. Kazempour, A. Hasanabadi, F. Nosouhi, Martine Pithioux, et al.. Influence of
bone microstructure distribution on developed mechanical energy for bone remodeling using a sta-
tistical reconstruction method. Mathematics and Mechanics of Solids, SAGE Publications, 2019,
pp.108128651982841. �10.1177/1081286519828418�. �hal-02042582�
Mathematics and Mechanics of Solids 1–15
ÓThe Author(s) 2019 Article reuse guidelines:
sagepub.com/journals-permissions DOI: 10.1177/1081286519828418 journals.sagepub.com/home/mms
Influence of bone microstructure
distribution on developed mechanical energy for bone remodeling using a statistical reconstruction method
Aerospace Engineering Department, Iowa State University, Ames, IA, USA
School of Mechanical Engineering, College of Engineering, University of Tehran, Tehran, Iran
Mechanical Engineering Department, University of Birjand, Birjand, Iran
School of Mechanical Engineering, College of Engineering, University of Tehran, Tehran, Iran
University of Aix-Marseille, APHM, CNRS, ISM, and Sainte-Marguerite Hospital, Institute for Locomotion, Marseille, France
School of Mechanical Engineering, College of Engineering, University of Tehran, Tehran, Iran
University of Strasbourg, CNRS, ICUBE Laboratory, Strasbourg, France
University of Strasbourg, CNRS, ICUBE Laboratory, Strasbourg, France
Received 30 October 2018; accepted 12 January 2019
Daniel George, University of Strasbourg, CNRS, ICUBE Laboratory, Strasbourg, France.
The development of a predictive model for bone remodeling is becoming increasingly important for medical applications such as bone surgery or bone substitutes like prostheses. However, as bone remodeling is a complex multiphysics phenomenon and difficult to quantify experimentally, predictive numerical models remain, at best, phenomenologically driven. Patient dependency is often ignored as its influence is usually considered secondary, although it is known to play an important role over long periods of time. Another difficulty to study this patient dependency is the availability of experimental samples to carry out extensive analyses. Using our recently developed statistical reconstruction framework, a set of ‘‘bone like’’ microstructures with variety of distributions has been created to study pseudo ‘‘patient variabilities.’’ The method provides similar effective stiffness tensor, equivalent stresses, and strain energy distributions for the original and the statistically reconstructed samples. The main out- come of this study is the correlation of similar effective mechanical properties between samples when bone remodeling will depend on the local strain energy distribution as a function of each bone microstructure. It is expected that two different micro- structures with equivalent bone volume fraction will lead to identical bone remodeling in a short period of time, whereas this needs to be proven for long term evolution. This work could be used to develop precise predictive numerical models while developing parametric studies on an infinite number of virtual samples and correlating patient dependency with more precise mechanobiological numerical models.
Bone microstructure, statistical reconstruction, finite element model, mechanical behavior
It is well established in the literature that the interaction between mechanics and biology plays a crucial role in the interpretation of growing tissue behavior [1–3]. This mechanobiology depends on the natural tendency of the biological tissue to develop optimizing behavior to gain proper mechanical strength with the minimum amount of material. For bone adaptation and remodeling, this optimization problem is at the origin of many studies since the early work by Wolff  followed by many others [5–9] exploring the internal architecture and external conformation of bones changes in accordance with mathematical laws.
The evolution of bone microstructure being dependent on cells and microstructure distribution, various mechanical stimuli have been proposed to trigger bone adaptation [10–13]. While continuum models, for the description of natural bone regeneration, are widely spread in the scientific literature, scale related effects of the material, are not often integrated in the structural evolution due to its highly heterogeneous nature at the small scales. At these scales, the classical continuum theory does not allow to describe the correct material behavior where the prediction made by Cauchy continuum theory starts being far away from the experimental evidence [14–18]. Hence, adequate homogenization methods [19,20] need to be developed in order to integrate all these local phenomena at the global scale.
Historically, bone mechanical behavior was dealt with using classical optimization processes based mainly on the developed mechanical strain energy density (SED) through the material [21–29]. However, to be able to obtain a good predictive numerical model, the biological phenomena  need to be linked with the surrounding physics [31–35], and account for the growing capillaries and nutrient supply [36–39].
Lately, a new form of mechanobiological stimulus for bone remodeling has emerged integrating coupled biological and mechanical effects accounting for cell migration and the nutrient supply chain [40–42].
Although this allows accounting for the couplings between the mechanics and biological phenomena, it remains a macroscopic approach and requires more insight about the locally occurring mechanobiology.
Bone microstructure distribution is optimized in order to sustain the externally applied mechanical loads and its evolution changes over the long term as a function of local biological information.
However, on a macroscopic scale, where the bone density is characterized only as a homogeneous
media, the influence of this microstructure over the long term remodeling kinematics is little investi-
gated. Although some numerical models tried to predict the bone remodeling kinematics from known
trabecular bone distributions [43–46], these do not provide insight about long term evolutions. In addi-
tion, patient dependent bone microstructure is very variable [47,48], this could impact directly the
numerical model predictions. Lately, some numerical models have investigated the correlations between
the bone stiffness and simplified microstructure distribution [49–53] through multiscale homogenization
procedures. However, the bone remodeling processes accounting for these microstructure variabilities at
the macroscopic scale are not studied since these works are mostly related to the structural mechanics homogenization process.
The ultimate goal of this research is to study the influence of the local bone microstructure distribu- tion on the macroscopic bone density evolution over long periods of time. The first step of this study require an adequate method for bone microstructure reconstruction in order to study large sets of speci- mens as it is not possible to extract that amount of real bone samples, and show that the proposed recon- struction method is able to provide corresponding results with different structural samples as equivalent effective stresses, strain energy and stiffness tensor. For this, we present here a methodology to study the influence of the bone microstructure distribution on the developed mechanical energy field. Real bone microstructures are extracted from computed tomography (CT) scan data and segmented/reconstructed to obtain the corresponding finite element (FE) numerical model. A statistical method is used to recon- struct several equivalent bone microstructures with identical homogeneous stiffness. FE models are then constructed from these statistical microstructures. The same mechanical loads are applied on the differ- ent FE models to extract the variabilities of the local SED that will be at the origin of the bone remodel- ing kinetics.
2. Experimental details 2.1. Specimen preparation
The real bone specimen was extracted from the femur of an 85-year-old woman post mortem. The adult bone was harvested from the corpse at the Timone Hospital (Marseille, France). The specimen was cut into a parallelepiped rectangle of length, width, and thickness dimensions 9.88 mm, 6.13 mm, and 2.29 mm, respectively, using a water-cooled low-speed diamond saw (Buehler Isomet 4000, Buehler, Lake Bluff, IL, USA). The length of each specimen was measured with a digital calliper (Absolute digimatik solar, Mitutoyo, Kanagawa, Japan, measurement error of 0.03 mm). The specimen was stored under vacuum at 220°C.
2.2. Image acquisition
The specimen was imaged at 5.5 mm voxel size using a micro-CT system (Phoenix Nanotom 180 S, General Electric, Germany). The scanning was done with a hydrated bone specimen, immersed in salt water inside a 25 mm inner diameter plastic tube. The axial specimen main axis (i.e., Haversian canal’s principal orientation and medullar canal orientation) was aligned with the rotational sample holder axis. Scans were done with a field of view of 2284 × 2304 pixels, with a maximum voltage source of 90 kV, a current of 120 mA and a rotation of 360° providing 2400 projections per scan. The exposure time was 500 ms with a total scan time of 85 minutes. The bone density was measured at 92% of the overall specimen volume.
3. Theoretical modeling
The statistical reconstruction approach enables to obtain various different microstructures with identical effective stiffness tensor by exploiting a single cut section image through the original bone sample. Bone images can be extracted from CT-scan or other experimental techniques.
Following our previous works [54,55], several bone microstructures were generated with identical effective stiffness tensor to evaluate the effect of the geometrical distribution of bone microstructure on local energy. This enabled to study many different scenarios (different virtual samples), using the full spectrum of two-point correlation function (TPCF) for eigen microstructure, without the need of extracting real bone samples.
The characteristic function (CF) of the heterogeneous microstructure can be written  as:
= 1 if s 2 phase n 0 otherwise
where n is a specific phase and the s index enumerates the voxel number of the sample.
This method is based on the fact that the material is not a functionally graded material (FGM) and that the statistical information of parallel cut sections are identical.
To reconstruct a three-dimensional (3D) representative volume element (RVE) based on given two- dimensional cut-sections, we introduce TPCFs, being statistical functions that give some information about the volume fraction, shape and distribution of the microstructure phases and are correlated with its various features such as effective thermal and mechanical properties .
In this research, we use fast Fourier transform (FFT) and a phase recovery algorithm to reconstruct the microstructure . The TPCF of the phases n and n0
, for an arbitrary vector t, can be defined as
(t) = 1 S
where S is the number of all voxels in the RVE and t is an arbitrary vector selected from the RVE. The Fourier transform (FT) of equation (2) leads to a more convenient form  for computation:
= F Cnn
= 1 S
Using the variable exchange (t = z s) and assuming a periodic extension of the RVE in all directions, equation (3) can be written as
= F Cnn
= 1 S
S j K bmn
j K bn
where j K bmn
j and unm
are the module and phase of the FT for the CF, with K bmn
= F kns
= j K bmn
ð5Þ It should be noted that the FT, expressed as F ð Þ, is calculated over all axes (i.e. 3D FT for : (s1
In equation (3), if n = n0
the TPCF is also called autocorrelation function, and its FT, using equation (4), can be obtained as
S j K bmn
Equation (6) shows that the FT of the autocorrelation function is related only to the FT module of the CF. If the FT of the autocorrelation functions exist, it is then possible to calculate its modules. Hence, for a two-phase microstructure, if the autocorrelation functions are to be known at first, it is possible to reconstruct the microstructure if the phase of the microstructure (i.e. unm
) is determined (see equation (5)). The reconstruction of an object based just on its FT modules, called phase recovery , is a com- mon method in astronomy and microscopy.
The application of this procedure for microstructure reconstruction was first introduced by Fullwood et al. . The reconstruction procedure using the phase recovery algorithm is as follow:
(1) Based on the known autocorrelation functions, the module of the CF is calculated using equa- tion (6). It is called the original amplitude. From this first step a random microstructure is generated.
(2) Once the FT of the randomly generated microstructure calculated, its amplitude is replaced by the original amplitude and then the inverse FT is calculated.
(3) Constraints of the generated microstructure are applied. If the difference between the FT ampli-
tude of the obtained CF and the original amplitude is below a given threshold, the reconstruction
procedure is considered completed and acceptable. Else, the obtained CF is defined inadequate
for this generated microstructure and the procedure is reset until the difference between the two amplitudes falls under the given threshold.
An improvement of this method was recently proposed by Hasanabadi et al. [54,55] on a new approxi- mation for the calculation of the TPCFs for a 3D RVE. We assume that the TPCF of an identical vec- tor in a given RVE in two parallel planes are approximately equal. Hence, only two perpendicular cut- sections (planes) in the RVE are necessary for the TPCFs definition and reconstruction process. This assumption is valid for statistically homogenous media . As shown in Figure 1, an arbitrary vector r in space can be decomposed into rz
. If the TPCFs of two planes, xy and yz are known, the full set of TPCF for 3D RVE can be approximated  based on
ð Þ’ r C211
is the volume fraction of phase 1.
The flowchart of the reconstruction procedure is presented in Figure 2. More details of this method can be found in .
In this approach, TPCFs were extracted using CT images and used to reconstruct microstructures converging to the real ones. The main reasons to choose this reconstruction technique are as follows:
(i) A strong contrast expansion shows that the stiffness tensor is linked to the TPCF of the micro- structure; therefore the TPCF is a very good selection of the statistical distribution descriptor.
(ii) In the phase recovery algorithm, different sets of TPCF can be employed for the reconstruction procedure, therefore enabling to reconstruct a variety of microstructures with few cut-section images.
Decomposition of the vectorr
Flowchart of the reconstruction procedure.
An improvement of the reconstruction process is envisaged in future works using two-point cluster func- tions but the mathematical framework for this needs to be developed.
4. Finite element model
The original CT scanned images were cropped into size 351 × 319 pixels and were imported into the VCAT software (released by V-CAD Program, RIKEN, Japan). The images were then assembled into stacks of 150 images after thresholding and made a 3D RVE of the bone microstructure. Figure 3 shows the 3D RVE for the real bone specimen and the statistical one possessing similar realistic features (size, shape, and distribution) as the real one, being suitable for the calculation of its mechanical properties.
Figure 3 also shows the connected network of voids inside the cortical bone. Effective properties were extracted directly from the results of the FE analysis on statistical and real bone microstructures. A direct comparison was made between the real bone sample and statistical reconstructed ones to validate the reconstruction process.
In this work, the primary goal is to focus on the ability of the statistical reconstruction method to pro- vide ‘‘bone like’’ microstructures and check whether these reconstructed microstructures show similar mechanical characteristics as the real bone. Once the statistical reconstruction method validated on a number of samples, it is then possible to create virtually an infinite number of microstructures showing different microstructures distributions and bone densities, hence enabling to study an infinite number of
‘‘bone samples’’ without the need of specimen extraction. Although the computation time is an impor- tant aspect, this is not the primary focus here as it can be addressed in future studies, but rather crucial to validate the quality of the reconstruction method in the first place.
The V-CAT software was used with its built-in mesh generator to obtain a high quality tetrahedral FE mesh, accounting for highly irregular and high aspect ratio solid and void clusters. This capability enabled to preserve a good quality of the void volume fraction during the meshing process. The mesh simplifier software has been used to reduce the number of elements in the bone part without sacrificing the volume fraction of the void. The total number of elements in the bone part was around 3.5 million tetrahedral ele- ments for all RVEs. The volume fraction of the void phase has been calculated around 8%, which is very close to the original CT scanned data. More details about creating the 3D model, mesh generation and homogenization process for real and reconstructed microstructures are provided in .
The real internal bone microstructure either cortical or trabecular is subjected to the combination of normal and shear loads defined by the external bone geometry and load conditions (muscles, body weight, bone type). However, it is rather difficult to extract quantitative data from such conditions.
Hence, in order to be able to validate the statistical reconstruction method by comparing developed stresses and elastic strain energy on real and statistical bone microstructures, we conducted six simula- tions (three tensile tests and three shear tests) on each RVE using the FE software ABAQUSÒ
. These were used to find the modulus of elasticity and Poisson’s ratios of the RVEs in the X, Y, and Z directions.
Finite element mesh for cortical bone microstructures (left: bone phase, right: void phase): (a) real specimen; (b)
statistically reconstructed specimen from cut section 2. The approximate size of samples (real and reconstructed ones) is 1930 x
1750 x 600mm3
Since bone is a highly heterogeneous material [61,62] and this affects its overall mechanical behavior [63,64], it is necessary to compare the obtained results at the effective macroscopic scale. Based on these tests, stiffness tensors of all RVEs were obtained and influences of the microstructure distributions were quantified.
5. Results and discussion
Five statistical bone microstructures were reconstructed (see example in Figure 3). From these different cases, including real bone sample, homogenized macroscopic stiffness coefficients (i.e. Young modulus and Poisson’s ratio) were extracted for the validation of the reconstruction process, assuming the mate- rial (bone solid phase) mechanical behavior was linear elastic with a Young modulus E = 15 GPa (aver- age value for cortical bone) and Poisson’s ratio n = 0.3. The results are presented in Table 1. The real bone sample presented values of Young modulus varying between 11.17 GPa and 12.89 GPa, and Poisson’s coefficients between 0.228 and 0.301 in the different directions. It is observed that the Young moduli Ex
are the lowest and Ez
is the highest which is due to the fact that cortical bone micro- structure is orientated along the Haversian canal. Comparing these values with the obtained homoge- nized coefficients of all statistically reconstructed cases, it was observed that for all of them, the obtained Young moduli are very close to the minimum value obtained for Ey
of section 6 at 10.76 GPa and high- est value for Ez
of sections 2 at 13.326 GPa. The errors developed from the microstructures variations for the Young moduli are; for the minimum Young modulus value equal to 3.1%, for the maximum Young modulus value equal to 3.38% and for the range min-max equal to 4.39%. For the Poisson’s ratio, their variability checked between 0 and 0.06, which is a very small range. In addition, it was observed that the real sample mechanical properties are mostly situated in the middle of all reconstructed cases which show a good correlation with the different scenarios.
From the original bone sample, it was possible to reconstruct different bone microstructures corre- sponding to different case scenario (different samples/different virtual patients) with a very good accu- racy. The reconstruction method allows obtaining an infinite number of virtual cases (patients) from the real bone sample, to study their mechanical behavior individually, and compare them with the real bone sample. It is also possible to extract tendencies with given scenarios of specific microstructure distributions.
Once the statistical reconstruction of different microstructure was validated, both tensile and shear mechanical loads were applied on each of them to compare their mechanical behavior, as well as the stresses and energy/energy density distribution fields developed. Each model is constituted of about 3.5 million tetrahedral FE elements in the solid phase. The applied load corresponds to an average standing person body weight (about 750 N) downscaled to the size of the sample surfaces. This leads to small deformation in the sample for the given mechanical properties; hence linear elastic analysis is adequate here. For the sake of lightness of the paper, we present only the results of the real bone sample with two other statistical microstructures built from cut section 3 and cut section 5 on the real bone sample respectively.
For the tensile test, the stresses are plotted in the corresponding loading direction (x) and (z), together with the corresponding SED developed within the microstructures. They are presented in Figures 4 and 5, respectively. For the shear load scenario, stresses in the (xy) direction together with SED are presented in Figure 6. Although the effective equivalent mechanical properties are similar for all cases (see Table
Modulus of elasticity and Poisson’s ratio in different directions for the real and statistical bone microstructures.
(GPa)nxy nxz nyz nyx nzx nzy
Real bone 11.723 11.172 12.894 0.228 0.263 0.262 0.275 0.289 0.301
Cut section 2 12.506 12.064 13.326 0.291 0.272 0.274 0.281 0.29 0.301
Cut section 3 11.456 11.310 12.686 0.281 0.260 0.264 0.277 0.288 0.298
Cut section 4 11.456 11.310 12.713 0.281 0.260 0.264 0.277 0.289 0.297
Cut section 5 11.556 11.229 12.838 0.288 0.259 0.263 0.279 0.288 0.297
Cut section 6 11.185 10.765 12.370 0.282 0.259 0.258 0.271 0.287 0.298
1), the stresses and SED, presented in Figures 4 to 6, show different distributions for both tensile and shear applied loads. Despite this anisotropic distribution, the amount of developed energy within the samples remains similar (see below).
The interpretations of these results tend to show that:
(i) The statistical reconstruction method provides a practical method to study any virtual sample from the mechanical behavior point of view as homogenized mechanical variables (stiffness coef- ficients, stresses, and strain energy) remain very similar. It provides a viable method to extract local microstructures interpretations. More specifically, it shows the equivalent correlation
Developed stresses and strain energy density in the real bone and statistical samples (section 3 and 5) under tensile load applied in thex-direction.
Developed stresses and strain energy density in the real bone and statistical samples (section 3 and 5) under tensile load
applied in thez-direction.
between homogenized bone density measurements (as in magnetic resonance imaging informa- tion, for example, for the gray scale of the Hue value) and different types of microstructure distributions.
(ii) The variabilities of the mechanobiological response for each reconstructed case can be evaluated as a function of the distributed SED and the different microstructure distributions. This in turn can provide long term variations in the bone density evolution and can show the influence of each of the different microstructures on the bone density kinetics.
To evaluate the potential bone density evolution as a function of the applied mechanical loads, the total developed strain energy inside each sample for the different cases (real sample and five reconstructed cases) in tensile and shear load conditions are presented in Figure 7.
Small variations of the developed strain energy are observed for each of the different load scenarios.
For tensile loads, the strain energy varies from a minimum of 1.485 mJ/mm3
up to 1.786 mJ/mm3
. For shear loads, it varies from a minimum of 2.284 mJ/mm3
up to 2.622 mJ/mm3
. For all cases, the real
Developed stresses and strain energy density in the real bone and statistical samples (section 3 and 5) under shear load applied in thexy-direction.
0.0 0.5 1.0 1.5 2.0 2.5 3.0
X Y Z XY XZ YZ
Strain energy (mJ)
Real secon 2 secon 3 secon 4 secon 5 secon 6
Total developed strain energy for the different bone microstructures (X, Y, and Z indicate tensile test and XY, XZ, and
YZ indicate shear tests).
bone sample is always around the mid-value of the statistical cases in the same way as was observed for the stiffness coefficients. The strain energy variation for all cases is within 3% to 6% compared to the real bone sample showing the reliability of the statistical reconstruction method. The developed strain energy in the z direction is slightly higher than in the x and y directions for tensile load conditions. This is in agreement with the higher stiffness of the z direction reported in Table 1. However, interestingly, shear load cases show significantly higher strain energy than simple tensile load conditions. The average energy for shear load has increased by 53% compared to tensile load conditions. This needs to be inves- tigated in future work with a more exhaustive screening of different bone microstructure in order to extract the coupling effects between shear and tensile load conditions.
Nevertheless, as bone cells activation will depend on the developed mechanical energy within the structure, we can assume that for different types of bone microstructures, this coupling effect (between shear and tensile loads) will impact on the bone remodeling process. If shear stresses show to be predo- minant, it could be correlated to the fact that cells are more sensitive to shear load conditions than hydrostatic pressure , hence favoring shear loads for optimized bone reconstruction.
In order to correlate the viability of the reconstructed microstructures to the real bone sample, prob- ability distribution functions (PDFs) were extracted. It represents the number of elements in the sample having a specific strain energy and is plotted as an element count versus strain energy divided by the total number of elements in the model. Figure 8 shows the average PDF value of the statistically recon- structed cases with the real bone PDF distribution. Statistical variations are small and a very good agree- ment is observed between the reconstructed cases mechanical response and the real sample.
Since mechanical load type, load direction and microstructure distribution impact directly the bone density evolution, the SED for all the elements in each RVE were extracted. The PDFs of the SED for each load case and microstructure are presented in Figure 9.
For each load case, the PDF of real bone is plotted in red. We observe that not only the overall mechanical response of the statistically reconstructed microstructures is similar to the one of real bone but also the distributions of strain energy densities are similar. The variabilities observed in these results are based on the fact that a 3D stochastic reconstruction technique has been used for reconstruction of the bone microstructure. The proposed method includes two steps: (i) a full set of TPCFs is approxi- mated using correlation functions being extracted from two perpendicular images; (ii) the full set of approximated TPCFs are used to reconstruct microstructures using a phase recovery algorithm. Hence, the accuracy of the reconstructing technique can directly be related to the approximation of the full set of TPCF. In our previous study , it was showed that for anisotropic microstructure, the error of the estimated TPCF and consequently, the error of the reconstruction procedure increased in the direction with high anisotropic distribution of microstructure. In addition, the reference image used for the recon- struction is the source of errors as it depends on the approximated TPCF in the direction perpendicular to the microstructure distribution of the reference image .
Nevertheless, accounting for the anisotropic complexity of the trabecular bone microstructures, the differences obtained from the reconstruction method remain small, as presented in Table 2. Comparing these results with those in Figure 9 shows that:
(i) All strain energies over the whole sample for the statistical cases remain lower than 10% varia- tions compared with the real bone sample. For simple tensile load cases, variations were between 0.2% and 4.5%, showing the influence of the anisotropic microstructure distribution over the reconstruction method . For shear load cases, the differences were up to 9.4% in the yz direc- tion showing in addition to the statistical error the sensitivity of the shear load scenario on the microstructure distribution, as presented on Figure 7.
(ii) For the standard deviation variations, they are not correlated to the strain energy variations as the mean strain energy does not account for the individual microstructure distributions.
However, we can still observe that for tensile cases, the z direction shows higher difference due
to the stiffness difference with other directions and reconstruction method . This does not
appear in the shear load case as it is a tangential load. The full width at half maximum (FWHM)
deviations of the PDF for tensile load remain within the 10% variability. For the z direction, it is
Probability density function for the YY (a) and ZZ (b) tensile cases, and XY (c) shear case as a function of the developed local strain energy (mJ/mm3
Normalized probability distribution function of strain energy density for the different microstructures with different
mechanical load directions.
It appears from the results in Table 1, Figures 7 to 9, and Table 2 that the statistical reconstruction method enables to study virtually an unlimited number of samples (bone like microstructures) as the calculated effective mechanical properties are very similar to the one of real bone. Some improvements remain to be done as the distribution of the strain energy shows variabilities over the statistical micro- structures (up to 10%) due to the abilities of the reconstruction method to best adapt to the real bone microstructure. These variations need to be evaluated with their respective impact on the bone density evolution over long periods of time in future works.
Differences between real bone sample and averaged of statistical cases for: (i) strain energy density variation in different directions in tensile and shear load condition (X, Y and Z indicate tensile test and XY, XZ and YZ indicate shear tests), and (ii) standard deviation difference at full width and half maximum (FWHM) as a representative of the variation of the energy density of each element compared to the mean value.
Tension X Tension Y Tension Z Shear XY Shear XZ Shear YZ
Mean strain energy density variation (mJ/mm3
0.0186(1.8%) 0.0449(4.5%) 0.0021(0.2%) 0.0699(7%) 0.0138(1.38%) 0.0942(9.4%) Standard deviation
difference at FWHM
11% 10% 42% 6% 11% 7%
(i) (ii) (iii)
(i) (ii) (iii)
(i) (ii) (iii) (iv)
(i) (ii) (iii) (iv)